If you can't read please download the document
Embed Size (px)
Plastic_Processing_Data_Handbook/list.txtPlastic Processing Data Handbook\Appendix - 20.pdf Plastic Processing Data Handbook\Aux equipment - 17.pdf Plastic Processing Data Handbook\Blow molding - 7.2.pdf Plastic Processing Data Handbook\Blow molding - 7.pdf Plastic Processing Data Handbook\Calendering - 8.pdf Plastic Processing Data Handbook\Casting - 9.pdf Plastic Processing Data Handbook\Coatings - 10.pdf Plastic Processing Data Handbook\Compression and transfer molding - 11.pdf Plastic Processing Data Handbook\Extrusion - 6.2.pdf Plastic Processing Data Handbook\Extrusion - 6.3.pdf Plastic Processing Data Handbook\Extrusion - 6.pdf Plastic Processing Data Handbook\Foam molding - 11.pdf Plastic Processing Data Handbook\Forming - 12.pdf Plastic Processing Data Handbook\Front matter.pdf Plastic Processing Data Handbook\Fundamentals - 4.3.pdf Plastic Processing Data Handbook\Fundamentals - 4.pdf Plastic Processing Data Handbook\Index - 22.pdf Plastic Processing Data Handbook\Injection molding - 5.2.pdf Plastic Processing Data Handbook\Injection molding - 5.3.pdf Plastic Processing Data Handbook\Injection molding - 5.pdf Plastic Processing Data Handbook\Other processes - 16.pdf
Plastic_Processing_Data_Handbook/Plastic Processing Data Handbook/Appendix - 20.pdfAppendix
METRIC CONVERSION CHARTS
Metric to USUS to metric
Multiply byUSMetricMultiply byMetricUS
Ib inr3Ib fr3Ib fr3Ib in.'3
Ib inr3Ib fr3Ib fr3Ib in.-3
Temperature0.5561.80C + 321.8K- 459.67
1.8(0F -32)/(1.8)(0F + 459.67)7(1.8)
Energy and power0.73768.8500.01871.870.47550.73551.34190.000953.4126.9330.42990.00023925.4
ftlbfin.lbfftlbf in."1ftlbf in."1ftlbf inr2kWUS horsepowerBtuBtuBtu in. Ff1Ir20F1Btu Ib'1BtUIb-10F1V mir1
ftlbfin.lbfftlbf in.-1ftlbf inf1ftlbf in.-2kWUS horsepowerBtuBtuBtu in. h^fr2 0F1Btu Ib-1BtUIb-10F1V mil'1
Ib min"1Ib h-1
Source: National Bureau of Standards Metric Information Office.
Metric to USUS to metric
Multiply byUSMetricMultiply byMetricUS
inch3fluid ouncequart (liquid)gallon (US)gallon (US)foot3foot3yard3in.3 Ib-1ft3 Ib-1
ounce (avdp.)poundpoundpoundUS ton (short)
centimeter3centimeter3decimeter3 (liter)decimeter3 (liter)meter3
gramgramkilogrammetric tonnemetric tonne
centimeter3centimeter3decimeter3 (liter)decimeter3 (liter)meter3
gramgramkilogrammetric tonnemetric tonne
inch3fluid ouncequart (liquid)gallon (US)gallon (US)foot3foot3yard3in.3 Ib"1ft3 Ib-1
ounce (avdp.)poundpoundpoundUS ton (short)
Source: National Institute for Science and Technology, Metric Information Office.
Metric prefixes*Standard metric symbols
A ampere d m3bar bar mcd candela NC celsius3 Pag gram Sh hour sHz hertz tJ joule VK kelvin Wkg kilogram
Numerical value Term
a Formerly called centigrade.b These prefixes may be used with all metric units.
MATHEMATICAL SYMBOLS AND ABBREVIATIONS+-
~ SS> ^< ^J=.=
I lr 3/V / V
plus (addition)minus (subtraction)plus or minus, (minus or plus)times, by (multiplication)divided byis to (ratio)equals, as, so isthereforeequalsapproximately equalsgreater thanless thangreater than or equalsless than or equalsnot equal toapproachesvaries asinfinityparallel tosquare root, cube rootsquarecircledegrees (arc or thermometer)minutes or feetseconds or inches
a', a"U1, U2
OO, , (IZla
a\ a~2sin"1 an
a, Z8, e
a-prime, a-second0-sub one, a-sub two
parentheses, brackets, braces
angle, perpendicular tofl-square, 0-cubeI/a, I /a2the angle whose sine is api = 3.141592654+summation ofbase of hyperbolic, natural orNapierian logs = 2.71828 +differenceacceleration due to gravitycoefficient of elasticityvelocitycoefficient of frictionpressure of loadhorsepowerrevolutions per minute
GREEK ALPHABETA, aB, pr,yA, 8E,e^C
H, il0,e#1,1K, KA 7 A,M, JLl
N, vE, (pO,on,7iP, p^,CT, C,
T, TY, DO, X, X1F, \|/Q,co
PROPERTIES OF WATER
Density of water is 62.38 Ib ft"3 or 0.0361 Ib in."3Specific gravity of water is 1 gem"3lft3 of water at 39.10F (3.90C) equals 0.4335 Ib in."2 (ft high)1 in.3 of water weighs 0.576 oz1 gallon of water contains 231 in.3 or 0.13368ft3!gallon of water weighs 8.3356Ib at 620F (170C) (air-free, weighed invacuum)1 ft3 of water equals 7.4805 gallons; a cylinder 7 in. diameter and 6 in. highcontains 1 gallon of waterThe maximum density of water is at 39.10F (3.90C)The freezing point of water at sea level is 32 0F (O 0C)The boiling point of water at sea level is 2120F (10O0C)
Front MatterTable of ContentsAppendixMetric Conversion ChartsMathematical Symbols and AbbreviationsGreek AlphabetProperties of Water
Plastic_Processing_Data_Handbook/Plastic Processing Data Handbook/Aux equipment - 17.pdfINTRODUCTION
Many different types of auxiliary equipment and secondary operationscan be used to maximize overall processing plant productivity and effi-ciency. Their proper selection, use, and maintenance are as important asthe selection of the processing machines (injection molder, extruder, etc.).The processor must determine what is needed, from upstream to down-stream, based on what the equipment has to accomplish, what controls arerequired, ease of operation and maintenance, safety devices, energy re-quirements, compatibility with existing equipment, and so on. This chap-ter provides examples of this selection procedure and its importance inevaluating all the equipment required in a processing line.
The equipment can be used to maximize overall processing productivityand efficiency, and reduce fabricated product cost. They can cost morethan the base machine. Examples of equipment are shown in Figs 16.1 and16.2. They include the equipment listed in Table 16.1.
All inline equipment has to be properly interfaced so it operatesefficently. Much of the equipment used in the past did not properlyinterface, so operations were rather less efficient than they could havebeen. A set of rules have been developed that govern the communicationand transfer of data between machines and auxiliary equipment.
New-generation auxiliaries that are continually produced are meaning-ful contributors to plant productivity via greater reliability of operationand pinpoint equipment control. As an example, fluid chillers and tem-perature control systems are major beneficiaries of the computer revolu-tion. They become more energy-efficient, reliable, and cost-effective withthe application of microprocessor- and computer-compatible controls that
Silos Blending Injection molding
Sprue & runnerseparation Productionrate
Receiving Raw mat'landpackaging
PalletizeIn-processcontainers8 pallets/shift500 PCS/HR.9 CTN./HR.6 pallets/shift18 pallets/day
Shipping Finish productwarehouse Finish productpallet Finishpacking Hot stampfoil imprinter Hookinsertion In processstorage
Figure 16.1 This production line starts with upstream auxiliary equipment andcontinues through an injection molding machine to the downstream equipment.
Drying hoppersAutomate partsremoval
Process watercooling towersystems
Surge bins Plasticstrandpellets
Figure 16.2 Auxiliary equipment next to different processing machines: begin atthe top right end and work round to the bottom left.
Table 16.1 Auxiliary equipment used with plastics processes
Adhesive applicatorBondingCuttingDie cuttingDryerDust-recoveryFreezer /coolerGranulatorHeaterKnittingLeak detectorMaterial handlingMetal treatingMetering /feeding materialMold extractorMold heat /chiller controlOvenPeJ letizer/ dicerPrinting / marking
Process control for individual or allequipment
Pulverizing / grindingRecycling systemRobotic handlingRouterSawScreen changerSere w /barrel backupSensor /monitor controlSoftwareSolvent recoveryTesting / instrumentationTrimmingVacuum debulkingVacuum storageWater-jet cuttingWeldingOthers
can communicate with primary processing equipment. They provide pin-point control of liquid temperatures. Thus, they have become significantcontributors to productivity.
Within a plastic processing communication protocol cell there are twobasic types of auxiliary devices: (1) devices that require minimum con-figuration or minimum data (chillers, dryers, loaders, and so on), and (2)devices that require large amounts of configuration data or provide largeamounts of process data (robots, gauging /sensors, mold /die controllers,cutters, and so on).
A set of rules govern communication or transfer of data between com-puter hardware and /or software. When related to plastic processingequipment, communication includes reference to exchange of processcontrols, meeting standards, and following production schedules, activi-ties that permit the interchange of actions, e.g., between molding ma-chines and auxiliary equipment.
The information that is required to monitor and configure a manu-facturing operation is distributed among various units of auxiliaryequipment. This information is transferred to the central control. Commu-nication interfaces and communication protocols have been developed to
allow this information to be exchanged. Successful communication re-quires a durable interface and a versatile protocol. A communicationinterface must be mechanically and electrically durable. Mechanical dura-bility is achieved by suitable hardware attachments and cable strain relief.Electrical durability is achieved by suitable transceiver circuitry. Circuitrymeeting the requirements of ANSI RS-485 is ideal for half- and full-duplexprotocols. It is designed for use where more than one device may talk ata time. Less durable circuitry, such as RS-232 and RS-422, may fail if morethan one device talks.
In most processes, for either small or large production runs, the cost of theplastics used compared to the total cost of production in the plant may beat least 60%. The proportion might be only 30%, but it is more likely toexceed 60%; so it is important to handle material with care and to elimi-nate unnecessary production problems and waste. Where small-quantityusers or expensive engineering resins are concerned, containers such asbags and gaylords are acceptable; but for large commercial and customprocessors, these delivery methods are bulky and costly. Resin storage inthis form is also expensive.
Any large-scale resin-handling system has three basic subsystems:unloading, storage, and transfer. For a complete system to work at peakefficiency, processors need to write specifications that fully account forthe unique requirements of each subsystem. The least efficient compo-nent, no matter how inconsequential it may seem, limits the overallefficiency of the entire system. The guidelines presented here will helpone to specify material-handling systems from the time of delivery to theplant on to processing machines that will maximize both efficiency andcapacity.
Railcars can be unloaded in many different ways, but some supplierssimply recommend inexpensive, back-to-back, flexible-hose assemblies tounload them. To save time at the loading dock, one should use a station-ary-pipe manifold arrangement along the length of the rail siding withconnections about every 15ft (4.5m). Thus transport is achieved with oneshort-flex hose from car to car instead of by handling as much as 100ft(30ft) of heavy-flex hose. Labor and unloading time will be saved, and thepressure drops inherent in long, multiple-connection, flex-hose runs willbe avoided.
The easiest method of unloading uses a vacuum pump/dust collector,which can be located in the silo skirt. The pump induces a vacuum in theline, drawing resin from the railcar into a vacuum loader. When thevacuum loader fills, the pump stops, and the resin dumps into the silo.
This on/off batching effect keeps transfer rates relatively low, typically6000-7000 Ib rf1 (2700-3200 kg tf 1X If the manifold pickup is far from thesilo, the transfer rates will drop.
If unloading requires high speeds or transfer over long distances, oneshould consider a push/pull system; resin is pulled from the railcar bynegative pressure, then pushed by positive pressure to its final location.Some equipment suppliers recommend a one-blower system, but thatlimits transfer capacities, requires more work-hours, and can actuallydegrade resin through excessive heat transfer within the airstream. One-blower systems can also lead to line blockages, as they lack purgingcapabilities.
Another way to unload railcars and transfer resin to storage silos is touse a two-blower system. One blower handles railcar unloading throughnegative pressure; the other transfers resins to silos using positive pres-sure. Splitting up the unloading and transfer of resin between two blow-ers permits peak efficiency in each operation. An improper pressurebalance across a single-blower system could greatly reduce transfer ratesat a critical point in the system, making the single blower work harder,increasing the heat of the conveying air, and causing resin degradation,particularly for thermally sensitive resins.
A two-blower system times purging to virtually eliminate any lineblockages. With this arrangement, the pressure blower continues operat-ing to ensure complete transfer to silos, while the vacuum blower remainsout of the transfer loop.
Silos and other containers provide more than just a place to stow awayresins until it is ready for use; silos protect resins from environmentaldamage caused by excess moisture, atmospheric pollutants, and solarradiation. Moreover, silos should require a minimum amount of mainte-nance; they should not leak, nor should they introduce rust or othercontaminants in the resin. They should resist structural damage fromenvironmental corrosion.
There are three types of silo construction: (1) spiral, with silos fabricatedfrom spun aluminum; (2) bolted, with silos made of carbon steel, stainlesssteel, or aluminum; and (3) welded, also with silos constructed of carbonsteel, stainless steel, or aluminum. Silos intended for pellet storage usuallyhave 45 discharge cones at the bottom. Powders and hard-to-flow resinsusually have a 60 cone to guarantee that the cone angle is greater than theresin's angle of repose [I].
Each type of silo has advantages and disadvantages. Spirals require theleast maintenance. Bolted construction can cost less than spirals, but witherection costs that can be three times higher. Because rubber gaskets areused, bolted silos have a greater tendency to leak. Welded silos have thelowest manufacturing cost of all, but their installation could be problem-
Figure 16.3 Bulk resin handling leads to better production economics.
line Container tilter
Sequencing valveVacuum hopperGrinder
Vacuum power unit Material line
Figure 16.4 Close-up of material handling by different machines.
atic and costly. So it is important to study available storage systems inorder to choose the supplier best able to meet individual specifications.
If computer-integrated resin-handling systems are considered, onemust compare their operating procedures with one's process require-
ments. These process requirements describe the flow of resin and productthrough the system, which determines the system's electronic architec-ture. Pertinent considerations include batch versus continuous opera-tions, the type and number of conveying lines, resin storage anddistribution, quality control means and procedures, inventory control, thetype and quantity of process parameter sensors, the type and quantity ofcontrolled devices, modes (automatic, semiautomatic, manual, and/orshutdown modes), process information, process management controls,and centralized versus local operation (Figs 16.3 and 16.4).
Energy conservation is only one of many factors that should be consideredin the selection of an automated materials-conveying system (as well as allequipment used in the processing line). Fortunately, any steps taken tosave energy will also save money in most cases. The traditional argumentsfavoring the silo are savings on resin costs, labor savings through theelimination of handling bags and cartons, the saving of costly warehousespace, and energy savings. For example, if a plant used a large quantity ofresins and did not use silos, during the winter months bags or gaylordswould be delivered repeatedly through 'open' delivery doors, and warmair would be lost.
With automatic delivery from silos, all resin-handling lines are kept asshort as possible. There is no reason for lines to conform to the right anglesof the walls; they should follow a straight line from the resin's source towhere it has to be delivered. There are graphs from systems suppliers thatshow the relationship between the length of conveyor lines and powerrequirements. The graphs also show the horsepower required, based ondifferent factors, such as the length and diameter of the delivery pipe, theposition of the pipe, the type of resin being conveyed, the size of thehopper at the machine, and the rate of flow deliverable.
A graph will show, for example, that with an average pellet size of1^m., 351b/ft3 (560kgrrf3) bulk density, and a conveying vacuum of 12in.
of mercury (Hg), PE can be moved in different ways. With a 25 hp (19 kW)vacuum hopper unit, a line will convey 18 000 Ib h"1 (8200 kg h"1) of PE if itis only 100ft (3Om) long. Using the same power and a 450ft (137m) line,less PE will be moved. Suppliers' data will show the power required tomove a material in the fastest way with the least energy consumption. Toconvert energy consumption to electric-bill charges, one uses the follow-ing formula: 1 hp = 0.745 kW, 1 kWh = 3.6MJ = 3143 Btu.
With a long pipeline, a 25 hp (19kW) vacuum pump could be used. Ifthe line could be shortened, a 10 hp (7.5 kW) unit would convey the sameamount of plastic, resulting in power savings. One metre of vertical height
in the line equals 2 m of horizontal distance in its effect on conveying rates.Bends in the pipe add a considerable amount of equivalent footage.
If the lines cannot be kept short or relatively free of bends, then pressuredrops will exceed 12 in. Hg (4OkPa), requiring more power. Where thepressure drop is greater than 12 in. Hg (4OkPa), which is the normaloperating and limiting pressure for most vacuum systems, it is necessaryto use a positive pressure system. All these factors must be consideredinitially to obtain the best delivery system most economically.
The logic and approach used in materials handling also applies to the useof handling equipment to move processed parts. Parts-handling equip-ment (PHE) does not resemble the humanoids of science fiction. Robotsare blind, deaf, dumb, and limited to a few preprogrammed motions; butin many production jobs that is all that is needed. They are solutionslooking for a problem. Most plants can use some degree of PHE, and it cansubstantially increase productivity.
Use of PHE can range from simple operations, as reviewed, to rathercomplex operations with very sophisticated computer controls. Althoughthe concept of automatic operations is very appealing, the ultimate justi-fication for PHE (like material handling, process controls, etc.) must bemade on the basis of economics. At times it may provide the solution to
Table 16.2 Example of parts-handling equipment functions
ManualBoxConveyorUnscramble / orient
Not integrated with IMM function
Integrated with IMMSweepExtractorCavity separatorRobot /bang-bangRobot / sophisticated
Table 16.3 Example of parts-handling equipment growth rate
Percentage usedwith IMM
Box /collectorConveyorUnscramble / orientSweepExtractorCavity separatorRobot / bang-bangRobot / sophisticated
No. of moldcavities
sm, medanymedsm, medsm, medsmmedlge
Does notinclude PHE
25000-150000a sm = small, med = medium, lge = large.
'handling' a part that otherwise would be damaged. Tables 16.2 and 16.3provide information on PHE for injection molding.
CLEAN PELLETS AND PLANT
When plastics are extruded and pelletized, varying amounts of oversizedpellets and strands are produced, along with some fines. When the plas-tics are dewatered/dried or pneumatically conveyed, more fines, fluff,and streamers may be generated. In many cases, these 'problem products'must be eliminated, significantly reduced, or removed during processingin order to produce good-quality products. The process or product re-quirement may not be influenced, but with high throughputs, these inter-ferences can present all kinds of problems. Even if acceptable products areproduced, costs will be increased by the greater processing time, energyrequirements, process controls, and reject rate which result, and/or otherproblems that may develop.
Fines or dust are created when small particles are torn away from thepellet and hit a rough surface at high speed (rough pipe wall, etc.). Withsmooth pipe walls, the pellet will slide, generating frictional heat, andcould become sticky before it deflects (depending on the melting point).The pellet's surface can actually smear off, leaving a film streak on thesurface of the pipe. In time, this film can cover the whole inside of thepipe, and it can tear off in the form of fluff (short threads or hairlikeparticles) and subsequently streamers (long ribbonlike particles, also
called angel hair or snakeskins). In addition to causing dirty products, thestreamers can form into balls and create blockages through the rest of thesystem.
The entire action that produces these contaminants is based on a com-bination of conditions of heat, weight, and velocity. The first appearanceof fluff indicates that an operational threshold has been crossed. As condi-tions worsen, longer streamers form large quantities of this material.
These fines and other undesirable materials can cause a variety ofhandling and processing problems; so if they exist, they must be removed.Suppliers have different removal systems such as filters and cyclones.
Some in-plant systems, such as inline filters, are high-maintenanceitems. As the filter element fills, the pressure increases while the filteringsystem's efficiency decreases. The filter must be checked and cleaned on aregular schedule to maintain its efficiency.
To remove dust or fines, consider using a compressed-air, backwash-type filter/receiver. Electronically controlled pulsing jets effectively shakefines from filter media automatically, eliminating human error in main-taining the filter system.
The need for cleanliness of the pellets, as well as the plant, is easy tounderstand. No casual dirt or dust, contaminants, different compounds,metal chips, or other foreign matter can be tolerated. This type of care alsoprotects the processing equipment.
All plastics, to some degree, are infuenced by the amount of moisture orwater they contain before processing. With minimal amounts in many
Ambient conditions: 750F50% relative humidity(550F dew point)
Internalvaporpressure (dry) = +0Externalvaporpressure (550F d.p.) = - 0.214 psi
A P = -0.214psi
Figure 16.5 Moisture absorption: mechanics.
plastics, mechanical, physical, electrical, aesthetic and other propertiesmay not be affected, or may be of no consequence. However, there arecertain plastics that, when compounded with certain additives, couldhave devasting results.
There are also hygroscopic plastics which require special drying equip-ment (Chapter 1). It is interesting that moisture is a major problem whichhas continually influenced degradation of processed plastics. Even thosewhich are not generally affected by moisture can only tolerate a certainamount. (Day-night moisture contamination can be a source of problemsif not adequately eliminated; otherwise it has a cumulative effect.)
During the drying process (Fig. 16.5) at ambient temperature and 50%relative humidity, the vapor pressure of water outside a plastic pellet isgreater than within. Moisture migrates into the pellet, increasing its mois-ture content until a state of equilibrium exists inside and outside thepellet.
But conditions are very different inside a drying hopper with a con-trolled environment. (Fig. 16.6). At a temperature of 1770C (35O0F) and-40 0C (-40 0F) dew point, the vapor pressure of water inside the pellet ismuch greater than the vapor pressure of water in the surrounding air, somoisture migrates out of the pellet and into the surrounding airstream,where it is carried away to the desiccant bed of the dryer.
Before drying can begin, a wet material must be heated to such atemperature that the vapor pressure of the liquid content exceeds thepartial pressure of the corresponding vapor in the surrounding atmos-phere. The effect of the atmospheric vapor content on the rate of the dryeras well as the effect of the material temperature is conveniently studied byconstruction of a psychrometric chart (Fig. 16.7). It plots moisture content,
Hopper conditions: 35O0F(-400F dew point)Migrationoutward
Internalvaporpressure 35O0F = + 27.4
Externalvaporpressure (-4O0F d.p.) = - 0.002 psi
A P = + 27.4 psi
Figure 16.6 Moisture migration: mechanics.
Dry bulb temperature, 0CFigure 16.7 Psychrometric chart: air-water vapor at 101.3kPa (latm).
Table 16.4 Drying equipment for coaters
Heat transferConvection dryers
Parallel airflowImpingement airAirfoilThrough dryers
Infra-red radiation dryersNear infra-red (electric)Far infra-red (electric or
Idler-supported dryersConveyor dryersCatenary dryersU-type dryersArch dryersTenter frame dryersFloater dryers
dry-bulb temperature, wet-bulb or saturation temperature, and enthalpyat saturation.
More details about processing plastics are given in Chapter 1. Eventhough processes may differ in other respects, they often use similarprocedures for drying. Specific procedures and equipment for certainprocesses are given in Table 16.4.
FEEDERS AND BLENDERS
As with other process equipment, suppliers of dryers, blenders, and me-tering equipment are increasing the feeding accuracy of the equipment bythe incorporation of microprocessor-based controllers that can be easilyinterlinked with the computer facilities of the main plant. Most processorsdeal with a wide variety of resins and additives, including regrind andcolor concentrates. As the quality and cost of the product depend directlyupon how carefully processors measure and mix components, blendingrepresents a critical stage in material handling (such as meeting tightrequirements according to a target; see Fig. 1.36, page 102).
To mix components easily and economically, processors may use blend-ers mounted on machine hoppers. In this operation, which offers greatflexibility, precisely predetermined proportions of each ingredient flowinto a mixing chamber, which should discharge a very accurate mix. Thekey to process success lies in carrying it out precisely. To do this, feedersmeter by volume or by weight.
In volumetric blending, variable-speed metering augers feed multiplecomponents into the mixing chamber. A microprocessor provides accu-rate, repeatable programming and closed-loop control over the variable
speed of each metering auger. A single master speed control can alsoincrease or decrease throughput while maintaining the desired blendratios. Operators can calibrate the actual volume easily by occasionallydiverting the component to a sampling chute and weighing a sample fromeach auger. The microprocessor monitors auger speeds at regular inter-vals to maintain constant feed rates regardless of variations in the meter-ing torque.
Gravimetric blending improves accuracy and requires less operatorinvolvement in calibration, particularly in running processes where greataccuracy is needed. Metering by weight eliminates overfeeding of expen-sive additives. The principle of gravimetric feeding with throughput ormetered weight control is well established. Equipment suppliers canassure an accuracy of 0.25-0.50% for ingredient and blend-ratio set-points at 2a (two standard deviations). By comparison, volumetric andquasi-gravimetric blenders that use batch operation usually have accu-racy variations of 2-10% or more.
Each hopper is mounted on a separate weigh-load cell specially de-signed and isolated to minimize the effects of on-machine vibration andelectrical interference. This unique load-cell approach updates the con-troller with weight information so it can adjust the motor speed forany necessary blend corrections. If the bulk density of any componentchanges, the blend is not influenced, as the unit only works on weights.Controllers are also capable of refilling individual component hoppersautomatically with no mixing delays.
Gravimetric metering is particularly advantageous in coextrusion. Inmany cases it is not possible to continually determine the individual filmthickness or thickness profile of the product. This system offers a verysimple means of constantly maintaining the average thickness of theindividual films and the overall thickness at better than 0.5%.
This mixing and metering activity is part of the overall conveyingprocess within the plant. Conveying includes not only mechanical andpneumatic transport throughout the plant or within each individualprocessing line, but also filtration of the exhaust air and safety engineeringto prevent dust explosion. With so much mixing required, color changesare becoming increasingly frequent. Table 16.5 explains the advantages ofcoloring at the hopper throat. The processor should determine what isrequired and obtain equipment to meet his/her specification. An indi-vidual evaluation is the best basis for taking advantage of developmentsin processing lines.
Motionless mixers, also called static mixers, are used for melt process-ing and for mixing liquids to produce an almost homogeneous mix. Theseunits are mounted inline on the output end of processing machines,such as extruders (Fig. 3.7, page 222), injection molding machines, andpolyurethane mixing units. Their mixing elements, housed within a
Table 16.5 Comparison of central blending versus coloring at the hopper throat
1. If the color blend is not correct (partstoo light or more color than necessaryin the mix), the mix must be emptiedfrom the hopper and reblended, acostly and time-consuming process.Even then, parts may not have theexact depth of color you desire.
2. Although some parts, as a cost-savingmeasure, could be molded with lesscolor than others, the mixing ofseveral batches with different let-down ratios is generally consideredimpractical.
3. Conveying of blended material oftenproduces separation of the colorpellets from the natural material dueto the much heavier bulk density ofcolor pellets. The result is inconsistentcoloring of parts.
4. Normal machine vibration and flowpatterns in the hopper cause someseparation of the color pellets duringresidence time in the hopper. Again,the result is inconsistent coloring ofparts.
5. When a production run is over, anyinventory of blended material left inthe hopper must be held for use atanother time. Storage space,contamination, spillage, mislabelingand tracking of this valuableinventory are all problems.
6. When a production run for one coloris over, your hopper must be emptiedin preparation for the next color. Timeis lost. Sometimes material is lost. Ifhopper and conveying system are notadequately cleaned, colorcontamination and rejected parts willresult.
7. If your material must be dried beforeuse, the drying of color blendspresents many logistical problems:more driers, careful planning fortransition to the next color, cleanoutof dryers, etc.
1 . Adjustments to color are madewith immediate results. If moldedparts are light in color, you canmake an adjustment and see theresults in minutes.
2. Every molded part can be customblended while in production foroptimum color usage and costsavings. Settings are recordedand used for exact repeatabilityon future runs.
3. Material is conveyed withoutcolor; separation is not a factor.
4. Color is metered only as parts aremolded. There is no residencetime for separation to occur.
5. All inventory of blendedmaterials is eliminated. Unusedcolor is returned to the containerit came from, uncontaminated.
6. Color changes require noemptying of the main materialhopper. Production does not stop.Transition time to the new coloris several minutes.
7. You dry only natural materialwihout having to concernyourself about color changes.
barrel, are a series of welded plates arranged to divide the melt andredivide it several times.
Motionless mixers provide effective dispersion of colorants and otheradditives such as plasticizers, antioxidants, flame retardants, stabilizers,and fillers. Their target is to increase the quality of the melt by eliminatingany temperature gradients.
Most processing plants have to reclaim reprocessable thermoplastic scrap,flash, rejected parts, and so on. If possible, the goal is to eliminate 'scrap'because it has already cost money and time to go through the process;granulating just adds more money and time. Different types of granu-lators are available from many different suppliers, and selection of agranulator depends on factors such as the type of plastic used, the type ofreinforcement, and product thickness and shape (Fig. 16.8). There aresome units in which subsystem granulators incrementally reduce theplastic from a large size to the required small size.
An easy 'cutting' unit is required, to granulate with minimum friction,as too much heat will destroy the plastic. General-purpose types havedefinite limitations. Blending with virgin material definitely influences,
Figure 16.8 Granulator: different types are available; this one granulates blow-molded bottles.
Tensile strength (ASTM D638-72) Impact strength (ASTM D256-73) Per cent elongation (ASTM D1238)Ten
Polys ty rene
Scrap content. % Scrap content, % Scrap content, %
Figure 16.9 How regrind levels affect mechanical properties of certain plasticformulations, 'once through' and blended with virgin plastics.
Number of times molded(Heat history effects performances)
Figure 16.10 Regrind: potential effects on the performance of injection-molded TPmixed with virgin material.
and can significantly change, the melt processing conditions and the per-formance of the end product. Recycled material is denser and usually hasa variable-size regrind that could affect the product's properties, as shownin Figs 16.9 and 16.10.
Front MatterTable of Contents16. Auxiliary EquipmentIntroductionTypesCommunication ProtocolMaterial HandlingEnergy Conservation
Parts HandlingClean Pellets and PlantDrying PlasticsFeeders and BlendersGranulators
Plastic_Processing_Data_Handbook/Plastic Processing Data Handbook/Blow molding - 7.2.pdfmoisture, etc. These include containers for paints, paint thinners, lighterfluids, polishes, cleaning solvents, cosmetics, and toiletries. An example isthe fluorination surface treatment to provide a gasoline barrier when blowmolding with PE - a barrier to nonpolar solvents. A barrier is created bythe chemical reaction of the fluorine and the polyethylene, which form athin (20-40 nm) fluorocarbon layer on the bottle surface. Two systems areavailable for creating the layer. The in-process system uses fluorine as apart of the parison-expand gas in the blowing operation. With it, a barrierlayer is created only on the inside. The posttreatment system requiresbottles to be placed in an enclosed chamber filled with fluorine gas. Themethod forms a barrier layer on the inner and outer surfaces.
INJECTION BLOW MOLDING
IBM has three stages (Figs 4.20 to 4.22). The first stage injects hot meltthrough the nozzle of an injection molding machine into a manifold andinto one or more preform (test-tube shaped) cavities. An exact amount ofresin is injected around the core pins. Hot liquid from a heat control unitis directed by hoses through mold-heating channels around the preformcavity; these channels have been predesigned to provide the correct heatcontrol on the melt within the mold cavity. The melt heat is decreased tothe required amount.
The two-part mold opens, and the core pins carry the hot plastic pre-form to the second stage, the blow molding station (counterclockwise).Upon mold closure, air is introduced via the core pin, and the plasticblows out and contacts the surface of the mold cavity. Controlled chilledwater circulates through predesigned mold channels around the moldcavity (usually 4-1O0C), and solidifies the hot plastic.
The two-part blow mold opens, and the core pin carries the completeblown container to the third stage, which ejects the part. Ejection can bedone by using a stripper plate, air, a combination of stripper plate and air,robots, and so forth.
IBM can have four or more stations (stages). A station can be locatedbetween the preform stage and the blow-mold stage to provide extra heat-conditioning time. A station between the blow-mold stage and the ejectionstage can provide additional cooling and/or secondary operations, suchas hot stamping and labeling. A station between the ejection stage and thepreform stage can be used to see whether or not ejection has occurred, toadd an insert to the core pin, and so forth.
The process parameters in preform production that determine the qual-ity of the part are the injection speed, injection pressure, hold-on (packing)pressure, heat control of the preform, and melt mix (Chapter 2). Theprocess permits the use of resins that are unsuitable for EBM, specificallythose with no controllable melt strength such as PET, which is used in
Injecting preform Blow molding and ejectionFigure 4.20 Basic injection blow molding process.
carbonated beverage bottles (stretch blown). The information on blowingparisons, cooling, clamping, and shrinkage that was presented for EBM isalso applicable to IBM.
Several different methods of IBM are available, each with differentmeans of transporting the core rods from one station to another. Thesemethods include the shuttle, two-parison rotary, axial movement, androtary with three or more stations used in conventional IM clampingunits.
Precise dimensional control offers several important advantages. It pro-duces scrap-free, close tolerance, completely finished bottles or containersthat require no secondary operations. Neck shapes and finishes, internallyand externally, can be molded with an accuracy of at least 4 mil( lOOjiim). It also offers positive weight control in the finished productaccurate to +/-0.1 g. These close size and weight tolerances are importantfor compatibility with downstream operations such as filling bottles.
Multistation machines are used. As an example, with a four-stationsystem, the conditioning station enables production of parts with betterdimensional and physical properties, giving better utilization of machinetime.
PREFORM NECK RINGPARISON
PREFORM MOLDPREFORM MOLD STATION
BLOWN CONTAINERCORE PIN OPENING(BLOW AIR PASSAGE)
BLOW MOLDBLOW MOLDNECK RING
RECIPROCATING SCREW PLASTICIZER
BLOW MOLD STATION
Figure 4.21 A three-station injection blow molder.
BLOW MOLDBOTTOM PLUG
Figure 4.22 Injection blow molding: a complete cycle begins with injectionmolding of the preform followed by the blowing cycle.
In the past few years, new markets have been established by newmaterials developed especially for IBM. Cough-medicine bottles, oncemade of glass, have virtually become all PP. Other specially formulatedand compounded plastics include PVC homopolymers and PC.
Early IBM techniques, all two-position methods, were adaptations ofstandard injection molding machines fitted with special tooling. The pri-mary difficulty with all of the two-position methods was that the injectionmold and blow mold stations had to stand idle during part removal. Thisled to the 1961 invention in Italy by Gussoni of the three-position method,which uses a third station for part removal. By the late 1960s, the concepthad been developed by commercial machinery builders, and it forms thebasis for virtually all IBM today (Fig. 4.21). One or more additional sta-tions can be added for various purposes: detection of a bottle not strippedor temperature conditioning of the core rod, decoration of the bottlebetween bottle blow mold and stripping stations, or temperature condi-tioning or preblowing of the parison between parison injection and bottleblow mold stations. These high-speed machines mold to tight tolerances.Machines are available that have outputs of 50000 PET bottles per hour(8V2-202/5floz, 240-580 cm3 bottles).
STRETCHING/ORIENTING BMHigh-speed EBM and IBM take an extra step in stretching or orienting.Figure 4.23 shows stretched IBM; with EBM the stretching action is similarto this, as it occurs during compressed air inflation (Fig. 4.8, page 325). InEBM the parison, which is mechanically held at both ends, is stretchedrather than just blown. Stretching can include the use of an expanding rodwithin the IBM preform or an external gripper with EBM.
By biaxially stretching the extrudate before it is chilled, significantimprovements can be obtained in the finished containers, as described inChapters 1 and 3. This technique allows the use of lower-grade resins or
thinner walls with no decrease in strength; both approaches reduce ma-terial costs. Stretched BM gives many resins (mono- or bioriented) im-proved physical and barrier properties (Tables 4.8 and 4.9). The processallows wall thicknesses to be more accurately controlled and also allowsweights to be reduced.
Draw ratios used to achieve the best properties in PET bottles (typicaltwo- and three-liter carbonated beverage bottles) are 3.8 in the hoopdirection and 2.8 in the axial direction; they will yield a bottle with a hooptensile strength of about 29000psi (20OMPa) and an axial tensile strengthof 15 000psi (104MPa).
Stretch blow is extensively used with PET, PVC, ABS, PS, AN, PP, andacetal, although most TPs can be used. The amorphous types, with a widerange of thermoplasticity, are easier to process than the crystalline typessuch as PP. If PP crystallizes too rapidly, the bottle is virtually destroyedduring the stretching. Clarified grades of PP have virtually zero crystallin-ity and overcome this problem.
The stretch process takes advantage of the crystallization behavior of
Table 4.8 Volume shrinkage of stretch blow molded bottles3
Type of bottle PercentExtrusion blow molded PVCImpact-modified PVC (high orientation) 4.2Impact-modified PVC (medium orientation) 2.4Impact-modified PVC (low orientation) 1.6Nonimpact-modified PVC (high orientation) 1.9Nonimpact-modified PVC (medium orientation) 1.2Nonimpact-modified PVC (low orientation) 0.9PET 1.2
a Seven days at 8O0F (270C).
Table 4.9 Gas barrier transmission comparisons for a 24fl.oz (680cm3) containerweighing 40g.a
Rate (nfday'1)Type of bottle Oxygen (cm3) Water vapor (g)PET (oriented) 10.2 1.10Extrusion blow molded PVC 16.4 2.01Stretch blow molded PVC (impact-modified) 11.9 1.8Stretch blow molded PVC (nonimpact-modified) 8.8 1.33AtIOO0F(SS0C).
Inject preform Reheat preform
Stretch blow molding andejection
Figure 4.23 Stretch injection blow molding.the resin and requires the preform to be temperature-conditioned thenrapidly stretched and cooled into the bottle shape.
There are inline and two-stage processes. Inline processing is done on asingle machine, whereas two-stage processing requires either an extru-sion or an injection line to produce the solid parisons or preforms. Witheither type of process, a specific-reheat blow machine is used to producethe bottle. With inline systems, the hot, firm plastic preform or parisonpasses through conditioning stations that bring it down from the 'melt'heat to the proper orientation heat (Table 4.10). A rather tight heat pro-file is maintained in the axial direction. Advantages of this approachare that the heat history is minimized (crucial for heat-sensitive resins),and the preform or parison can be programmed for optimum materialdistribution.
With the two-stage process, cooled preforms or parisons are conveyedthrough an oven (usually using quartz lamps) which reheats them to theproper orientation heat profile. Advantages include minimization of scrap(for EBM, there being no scrap with IBM using either the inline or the two-stage process), higher output rates, and the capability to stockpile pre-forms or profiles and improve thread finishes (EBM). Inline stretch IBM,which offers more flexibility from a material view, does not give thedegree of parison programming available in EBM stretch. An extrudedparison can be heat-stabilized, then the parison is held externally andpulled to give an axial orientation while the bottle is blown radially.Another technique stretches and preblows the parison before completingthe blowing operation. In both operations, scrap is produced at the neckand the base of the bottle. The processes completely orient the wholebottle, including the threaded end; this neck orientation does not occurwith stretch IBM. With EBM, threads are finished postmolding.
Extrusion processes can also use programmed parisons and two sets ofmolds. The first mold is used to blow and heat-condition the preform,actually to cool it to the orientation heat. The second mold uses an internalrod to stretch and blow the bottle. With two-stage EBM, the preforms orparisons are usually open-ended. They are reheated then stretched bypulling one end while the other end is clamped in the blow mold. Mini-mum scrap can be produced, and the compression-molded threads pro-vide a good neck finish. This system utilizes a conventional extrusion lineand a reheat blow machine whose oven contains quartz lamps to providethe proper heat. (When used to heat the preform or parison, they rotate ina heat-profile-controlled oven to provide uniform heat circumferentially.)
As blow molds do not have to withstand high pressure, a wide selectionof construction materials is available. The ultimate selection will dependon a balance of the following factors: cost, thermal conductivity, andrequired service life. The more commonly employed materials for smallparts are aluminum and aluminum alloys, steel, beryllium copper
Table 4.10 Stretch blow molding processing characteristics
Stretch orientationMelt temperature temperature
MaximumPlastic 0F 0C 0F 0C stretch ratio
PET 490 250 190-240 88-116 16PVC 390 199 210-240 99-116 7PAN 410 210 220-260 104-127 9PP 334 168 250-280 121-136 6
(Be/Cu), and cast zinc alloys (Kirksite, etc.). Aluminum molds are excel-lent heat conductors, are easy to machine, can be cast, and are reason-ably durable, particularly when fitted with harder pinch blades and neckinserts (Table 4.11).
Molds with aluminum pinchoff areas could last 1-2 million cycles ifproperly set up and maintained. But most molds use Be/Cu and steelpinchoffs, providing more durability, and they can easily be repaired. Be/Cu is preferred because of its high thermal conductivity; steel is predomi-nantly used because of its wear resistance and toughness.
Although Be/Cu and Kirksite are better conductors of heat, aluminumis by far the most popular material for molds, because of the high cost ofBe/Cu and Kirksite's short life (soft zinc alloy). Aluminum is light inweight, a relatively good conductor of heat, very easy to machine, and lowin cost. A major disadvantage is that it is easily damaged, particularly if itis abused. Its potential porosity may easily be eliminated by coating theinside cavity with a sealer such as automotive radiator sealant.
Aluminum is used for single molds, molds for prototypes, and largenumbers of identical molds, as found on wheel-type blowing equipmentor equipment with multiple-die arrangements. (It is best to prototypeusing a material that the production mold will use to duplicate heattransfer conditions.) Aluminum may tend to distort after prolonged use.Thin areas, like pinchoff areas, can wear in aluminum.
Be/Cu molds are corrosion resistant and very hard when compared to
Table 4.11 Materials used in the construction of blow molds3
Beryllium copper23 RC-30165
3BHN - Brinell hardness; RC = Rockwell hardness (C scale).b Specific gravities (lbinr3) AI = 0.097, Be/Cu - 0.129-0.316, steel = 0.24-0.29.
aluminum, making Be/Cu the choice for PVC. However, it is about threetimes as heavy as aluminum, costs about six times as much per volume,has a lower thermal conductivity, and requires about one-third more timeto machine.
Thermal conductivity of the Be/Cu alloy is slightly poorer as well. Forpolyolefin blow molding, some mold makers have combined the materi-als by inserting Be/Cu into the pinchoff area of an aluminum cavity,thereby obtaining a lightweight, easy-to-manufacture mold with excellentthermal conductivity and hard pinchoff areas.
Unlike injection blow molds that are mounted onto a die set, all extru-sion blow molds are fitted with hardened steel guide pins and bushings.These guide pins ensure the two mold halves are perfectly matched. Theremaining hardware in the process, dies, mandrels, blow-pin cuttingsleeves, and neck-ring striker plates, are all made from tool steel hardenedto 56-58Rc.
In blow molding plastics that produce corrosive volatiles (PVC, nylon,acetal, etc.), it is necessary to employ corrosion-resistant steels or to useplating, even gold plating. However, platings can lead to reductions ofstrength and hardness, and damage to edges and surfaces can easilyoccur. With proper care, lifespans of 105 to 106 cycles can be expected. Steelmolds are used for continuous production and longer runs.
Hardening is not necessary, and chrome plating is not customary.For large-volume parts with a content of 4yd3 (3m3) and upwards,welded machined steel plate construction can be considered. Cast metal isof no value for the mold bases. Given the right care, the life of steel moldsis the longest, at over 108 parts per mold. Inserts subject to wear and tearhave to be refurbished or exchanged at intervals of 105 or 106 cycles (Table4.12).
Unfortunately, most BM molds do not yet provide the high level ofcooling that has been achieved for decades with IM molds. A greater effortis now being made to properly incorporate cooling channels in BM molds,to provide necessary and controllable heat transfer. CAD systems noware available for proper design of the molds. Internal cooling with liquidN2, CO2, or refrigeration and ice crystals can improve efficiency by up to50%.
Nearly all BM resins used to be commodity types (PE, PP, PVC, and PS),but engineering types have been used more recently. Typical heats usedfor blow molding some resins are given in Table 4.13. The polyolefins (PEand PP) and rigid PVC have proved to be the most suitable materials forblow molding. Its heat control and rheology allow PE to be processedrelatively easily. The thermal sensitivity of PVC and the reprocessing of
Table 4.12 Guide to selecting construction materials for blow molds3
Property Steel Aluminum Be/Cu Aluminum Kirksite Be/Cu
Pinch life 4 3 2 2 1 3Cavity life 4 3 4 2 1 3Surface finish 4 3 4 2 1 3Heat control 2 4 4 2 1 3Mold modifications 2 4 2 1 1 2High volume 4 3 4 2 1 2Mold lead time 2 3 2 4 4 3Low cost 2 3 1 4 4 3Prototype cost 1 3 2 3 4 3Complex shapes 3 4 3 3 2 2Moving mold parts 4 3 3 3 1 1
a4 = best, 1 = poorest.
the flash can cause several difficulties if not handled properly. In retro-spect, PVC in particular, which imposed important and high performancerequirements on the processing operation, imparted major impulses to thefurther development of EBM technology and provided the impetus for athorough engineering analysis of melt flow through the extruder andblow heads.
The wide diversity of products being manufactured makes it clear thatprocessing plants will have to solve logistical problems such as the sepa-ration of material cycles and the drying of materials, as has been done inthe standard extrusion and injection molding plants.
Most engineering resins are hygroscopic and therefore must be prop-erly dried before processing. Moisture generally has an adverse effect onthe melt viscosity, surface, and physical properties of the product. Toavoid these problems, resins must be dried, usually to a residual moisturecontent of 8floz (237cm3)
Best process for polyvinyl chloride;many resins can be used providedadequate melt strength is available
Much fewer limitations on partproportions, permitting extremedimensional ratios: long andnarrow, flat and wide, double-walled, offset necks, molded-inhandles, odd shapes
Low-cost tooling often made ofaluminum; ideal for short-runor long-run production
Adjustable weight control; ideal forprototyping
Figure 4.6 A single blow-molded part can often replace several different injection-molded parts; the blow molding depicted is a structural multilayer coextrusion.
Figure 4.7 An integral carrying handle for an injection blow molded product: (1)the precision 'neck' mold, including a solid handle; (2) the preformed core andblow pin; (3) the basic water-cooled bottle female mold; and (4) the injectionnozzle of the injection molding machine.
recycled scrap, and limited wall thickness control or resin distribution.Trimming can be accomplished in the mold for certain mold types, orsecondary trimming operations have to be included in the productionlines, and so forth.
With IBM, the major advantages are that no flash or scrap occurs duringprocessing, it gives the best of all thickness and material distributioncontrol, critical neck finishes are molded to a high accuracy, it providesthe best surface finish, low-volume quantities are economically feasible,and so on. Disadvantages are its high tooling costs, the current lack ofblown handleware (there is only solid handleware Fig. 4.7), it is somewhatlimited to relatively smaller blown parts (whereas EBM can easily blowextremely large parts), and so forth. Similar comparisons exist withbiaxially orienting EBM or IBM. With respect to coextrusion, the twomethods also have similar advantages and disadvantages, but mainlymajor advantages. IBM can process PET (mono- or multilayer), stretching
it into the popular two- and three-liter carbonated beverage bottles (Table4.2).
Auxiliary equipment used for molding support functions is no differentfrom the equipment used by other processes. However, the nature of theprocess requires the supply of clean compressed air to 'blow' the hot meltlocated within a mold. The air usually requires a pressure of 80-145psi(0.55-1 MPa) for IBM. EBM requires 30-90psi (0.21-0.62MPa). However,stretch blow molding often requires a pressure up to 580 psi (4MPa). Thelower pressures generally create lower internal stresses in the solidifiedplastics and a more proportional stress distribution; the higher pressuresare low when compared to conventional injection molding. The result ofthe lower stresses is improved resistance to all types of strain (tensile,impact, bending, environment, etc.).
EXTRUSION BLOW MOLDING
In extrusion blow molding the melted plastic is continuously extruded asa tube (called a parison) into free air. It is located between the two halvesof the mold (Figs 4.8 and 4.9). The melt flowing through the die can formdifferent cross sections with or without changes in the parison's wallthickness as it exits the BM die (Table 4.3). When the parison has reachedthe required length, a mold-mounted or shuttled device below the diecloses around the parison and air forces the plastic melt against the cavitywalls. A blow pin is inserted through the parison, permitting air to enter.The parison then cools against the mold cavity.
Unlike injection blow molding (IBM), flash is a by-product of the proc-ess which must be trimmed and reclaimed. This 'excess' is formed whenthe parison is pinched together and sealed by the two halves of the mold.
In addition to continuous extrusion, there is also the intermittent extru-sion, also called discontinuous extrusion. Both can have a diehead withone or more openings; so one or more parisons can be extruded intosingle- or multiple-cavity molds. For increased production output, multi-ple extrusion heads are used (Fig. 4.10).
With continuous extrusion, the extruded parison is continuouslyformed at a rate equal to the rate of part molding and moving the mold(Figs 4.11 and 4.12). The mold is moved away from the parison drop, andwhen more than one mold is used, another mold moves into position. Toavoid interference with the parison formation, the mold-clamping mecha-nism must move quickly to capture the parison and return to the blowingstation where the blow pin enters. More than half of all blow-moldedparts are made using the continuous extrusion method. This process has
Parison being extruded
Compressed air inflatesparison
Blown containerbeing ejected
Figure 4.8 Basic continuous extrusion blow molding process: A = parison cutter,B = parison, C - blow mold cavity, D = blow pin.
Figure 4.9 Typical phases in intermittent extrusion blow molding with accumula-tor in the die.
three different modes of operation: the rising method, the rotary wheel,and the shuttle.
With the rising method, the parison is continuously extruded above themold. When it reaches the proper length, the open mold rises quickly toclamp the parison and returns downward to the blow station so that theparison continues to extrude. After the part is blown and cooled, the moldopens, the part is removed, and the process repeats.
The rotary wheel uses 3-20 clamping stations, possibly more. The sta-tions are mounted to a vertical or horizontal wheel. A parison is pinchedin the mold, parts are molded and cooled, and a cooled part is removed,all simultaneously as the wheel rotates past the extruder. This methodprovides high production rates.
With the shuttle method, two molds are located under the extruder. Asthe parison reaches the proper length, one mold located under the parisonis clamped quickly, the parison is cut and shuttled quickly to its blowingstation. With this dual-sided machine, the other (opened) mold movesunder the parison drop. Thus, the molds alternately shuttle sideways(Fig. 4.10).
With an accumulator, the flow of the parison through the die is cyclical,permitting intermittent or discontinuous EBM (Figs 4.13 and 4.14). The
Table 4.3 Examples
Open-loop axialdie-gap control
Servohydraulicclosed-loop axialdie-gap control
of differently performing extrusion blow molding dies
Fixed die gap
Premanently profiled;preferred in die landarea
Can be permanentlyshifted laterally tocorrect parison droppath
Can be axially shiftedduring extrusion
As above, with greaterspeed, accuracy, andflexibility
Permanently ovalized diegaP
Settable adjustment of die-gap profile
Programmable ovalizationand shifting of die gap
Advantage I disadvantage
Simple; inexpensive; noadjustment facility
Fixed circumferentialwall-thickness change;time-consuming; complex
Compromise betweenrequired drop path andequal wall thickness
Equal circumferentialwall-thickness changepossible; no feedback
Equal circumferentialwall-thickness changepossible, with feedback
Fixed, unequalcircumferential wall-thickness change possibleaffects entire parisonlength
Settable, unequalcircumferential wall-thickness change possible;rapid optimization
Programmablecircumferential wall-thickness change possible,independent of parisonlength
connecting channels between the extruder and accumulator, as well as theaccumulator itself, are designed to prevent restrictions that might impedeflow or cause the melt to hang up (Chapter 3). Flow paths should havelow resistance to melt flow to avoid placing an unnecessary load on themelt.
To ensure that the least heat history (Chapter 1) or residence time isdeveloped during processing, the design of the accumulator ensures thefirst melt into the accumulator is the first to go out when the 'ram' literallyempties the accumulator chamber; the goal is to have the chamber totallyemptied on each stroke. Plastics that are not heat-sensitive permit somerelaxation in their heat history.
Figure 4.10 A multiple continuous extrusion head (three parisons) blow moldingthree containers simultaneously in a shuttle clamping system.
Intermittent systems fall into three classes: reciprocating screw, ram,and accumulator. The reciprocating screw units act much like the injectionmolding machines (Chapter 2). Plastic is conveyed and melted by thescrew turning. As melt accumulates at the front of the barrel, the screw ispushed backward. Once a sufficient quantity of melt is in the barrel, thescrew stops rotating and pushes forward (ram action) forcing the meltthrough a die to form a parison (Fig. 2.5, page 124).
The ram-type machine incorporates a screw that delivers melt into achamber. An accompanying piston then forces the molten material fromthe chamber and through the die (Fig. 2.3, page 123).
Core or pin
Figure 4.11 Side-fed or radial-flow head around the core; die-fed die with heart-shaped grooves.
Figure 4.12 Continuous blow molding head having a spider-supported core.
Accumulator heads, the most common, are used particularly formolding large parts. Accumulator heads, attached to the end of extruders,are designed to collect and eject a measured amount of plastic (Figs 4.9and 4.13).
Overlapping melt flow
Programming cylinderRamming cylinder
Melt ramMelt flow
Figure 4.13 An accumulator melt flow head.
Melt properties are of critical importance to BM; more so than for conven-tional extrusion. To a large extent they determine the quality achieved.The melt viscosity decides whether sagging or lengthening of a parisonduring extrusion from the die can be compensated, particularly innoncircular parisons (Fig. 4.15). Because engineering resins have so farbeen used mainly with IM, most processors attempt to use easy-flowing,low molecular weight IM-grade resins. But in BM, particularly EBM, theobjective is very different; the melt should be viscous and of high molecu-lar weight (high melt strength) (Chapter 1). This requirement also gener-ally ensures another important feature, better impact strength. The meltviscosity should be nearly independent of the shear rate and the process-ing heat.
ExtrudeParison Drop Shot Recovery
Blow Molding CycleFigure 4.14 Blow molder using an accumulator head.
In raw-material data sheets there are usually no characteristics thatindicate whether the resin is suitable for BM, or up to what limit anapplication is sensible. With increasing markets for these materials, moreuseful data sheets for all types of resins are becoming available.
Another important melt condition, extensibility, relates to how success-fully large blowup ratios can be met, and whether edges and corners canbe properly blown without thin spots. For ease of processing, there shouldbe a large difference between the processing heat and solidification heat.This characteristic has a particularly advantageous effect on the quality ofthe blown surface. The greater the difference, the longer the time the melthas to be shaped, resulting in better surface definition. With a large differ-ence, the contact of the parison with the surface of the mold is not influ-enced (or is affected very little). With little difference in the heatingprofile, uneven contacting of the mold can cause an uneven surface ap-pearance, uneven stress, and so on. Increasing the mold heat can offsetsome of the negative effects. Unfortunately a large difference in the heatprofile involves increasing the cycle time, but this increase can be mini-mized to meet quality production requirements with no rejects.
Figure 4.15 Noncircular blow mold die, with and without wall thickness dieshape (dimensions in millimeters).
Parison thickness control
The control and monitoring functions range from extremely simple onesto expensive complete microprocessor systems. Some machines use elec-trical relays that permit molding with inexpensive machines which do notrequire a very sophisticated maintenance shop or skilled operators.However, to produce good-quality parts at the lowest cost, machine sys-tems generally have to be more sophisticated, to meet any degree ofperformance.
Electronic parison programming is an effective way to control materialusage and to improve quality and productivity. The most commonmethod is orifice modulation (Fig. 4.16). The die is fitted with a hydraulicpositioner that allows positioning of the inside die diameter during theparison drop. The OD to ID relationshing of the tapered die orifice open-
Profilecontrol signal Valve driver
Servo valve/cylinder head
Figure 4.16 An accumulator head with programmable process controller; it con-trols the melt characteristics (interrelated with extruder performance), the rate ofmelt flow to form the parison, and the profiling thickness of the parison as itextrudes from the die.
ing is varied in a programmed manner to increase or decrease the parisonwall thickness.
Electronic parison programming utilizes an electronic unit, commonlycalled a programmer, that uses a closed-loop servosystem supplyingproper signals to control the amount, direction, and velocity of the move-ment of the hydraulic positioner. Programmers are designated by thenumber of program points available, usually 5-100.
In extrusion of a parison, especially a large parison, the wall thicknesswill vary as the weight of the resin increases, and it sags. Parison controlmay be helpful, but another method of minimizing wall-thickness varia-tions is to increase the pressure of the melt in the die, either by regulationof the barrel back pressure or possibly by pressure variations via a ramwhen an accumulator is used. But an even wall-thickness distribution onthe parison circumference and wall-thickness control in the longitudinaldirection are seldom sufficient to meet today's quality specifications. In-creasing requirements and ever more geometric shapes necessitate a par-tial wall-thickness adjustment, realized by shaping the flow channels inthe die. The wall thickness along the length can be controlled by theconventional programmers reviewed. Circumferential distribution is con-trolled by patented predeformation of the die ring.
Parison control requires a compromise between the desired net weightand the need to maintain a sufficient safety margin over a set of minimumspecifications, which include minimum wall thickness, drop speed, drop
strength, dimensional stability, and fluctuations in net weight. Most ofthese parameters can be directly affected by the molder's ability to controlthe parison wall thickness. The most common and practical way of doingthis has been to adjust the gap between the die and mandrel (Table 4.3).
For some resins, it is advantageous to maintain a constant shear rate atthe die orifice. Constant shear ensures the melt is uniformly stressed andproduces a uniform surface texture. To provide constant shear, an accu-mulator ram speed is controlled according to a predetermined profile. Asthe parison drop increases, the ram stroke increases. Electronic and me-chanical systems are being used with adjustments that are reproducible atspeeds of 2OnImXs'1. This action can be applied only when a torpedo headis used. An adjustable core 'plug' at the center of the torpedo moveslongitudinally and controls the orifice opening without changing the vol-ume of melt in the accumulator (Fig. 4.16). In a central feedhead with theouter die ring moving, the volume of the melt in the flow channel varies,making it difficult to control the speed of the flow.
Processing capability developments in the past involved commodityresins, as they were predominantly used. Now there is more focus onengineering resins. Overlapping the melt streams in accumulator heads toobtain uniform wall thickness distribution is now a more fundamentalrequirement. The available accumulator heads differ in their feed-channeldesigns and are frequently protected by patents; so one must be carefulwhen purchasing them. In a parison head, the melt is divided into sepa-rate streams by the mandrel or spiders. Weld lines form where the flowfronts reunite. As the parison is deformed differentially in BM, theseweld lines are potential weak sections in areas of extreme deformation(Chapter 2).
If it is necessary to minimize streaks, another factor must be considered.No oxygen should be permitted to reach the melt and cause oxidationduring downtime. A special die with an automatic shut off prevents thisaction. During downtime, the barrel heat should not drop lower than2O0C above the softening point, in order to prevent excessive volumecontraction of the melt.
Accumulators can provide special products, an example being clearstripping systems. Two separately extruded melts enter the head and fusetogether prior to exiting. Like overlapping layer formation of the parison,this feature also provides a positive way to strengthen weld lines.
A very important factor in EBM is the effective diameter swell of theparison. Ideally the diameter swell would be directly related to the weightswell and would require no further consideration. In practice the existence
Table 4.4 Average parison swell for some commonlyused plastics
Plastics Swell, present
HOPE (Phillips) 15-40HOPE (Ziegler) 25-65LDPE 30-65PVC (rigid) 30-35PS 10-20PC 5-10
of gravity, the finite parison drop time, and the anisotropic aspects (theparison has directional properties) of the BM operation prevent reliableprediction of parison diameter swell directly with the weight swell.After leaving the die, the melt - which has been under shear pressure -undergoes relaxation that causes cross-sectional deformation or swell.
Parison swell tends to be the most difficult property to control in effortsto produce low-cost, lightweight products. Diameter swell is easy to see;with the parison dropping, one may be able to see it actually shrink evenafter it stretches. If it is shrinking in length, the wall must be thickening,and the parison is heavier per unit length, a behavior known as weightswell. Table 4.4 gives swell action for some common plastics.
For a given die cross section, the weight varies in proportion to thedeformation. The time dependence and the increasing effect of weightwith increasing parison length cause a narrowing of the diameter and areduction in wall thickness from the lower end toward the die. Excessivelength and prolonged hanging may lead to collapse, even with the usualprocedure of providing some air pressure flow during parison formation.With this section, unlike the other processing methods, the characteristicsof the melt within and after it exits the die are extremely critical indesigning the die to suit the blow mold. A high melt strength is desirableto minimize this problem.
Diameter swell is an important processing parameter that must becontrolled for EBM of unsymmetrical containers and particularly withblown side-handle products. Resins with an excessively high diameterswell could experience curtaining and stripping problems (adherence tomold cavity). An inadequate diameter swell contributes to an increase inrejects for defective handles.
The pinchoff is a very critical part of the EBM mold, where the parison issqueezed and welded together, requiring good thermal conductivity for
rapid cooling and good toughness to ensure long production runs. Thepinchoff must have structural soundness to withstand the resin pressureand repeated closing cycles of the mold. It must usually push a smallamount of resin into the interior of the part to slightly thicken the weldarea. It also provides a cut through the parison to provide a clean breaklater when flash is removed.
Most molds use a double-angle pinchoff with 45 angles and a 10 mil(250|Lim) land (Fig. 4.17(a)). When the blown part is large relative to theparison diameter, the plastic will thin down and even leave holes on theweld line, requiring pinchoff (Fig. 4.17(b)). Using shallow angles (15) hasa tendency to force the plastic to the inside of the blown part, therebyincreasing the thickness at the weld line. A pinchoff with a dam (Fig.4.17(c)) also helps to solve problems. The depth of the flash pocket isrelated to the pinchoff and is very important for proper molding andautomatic trimming.
A gross miscalculation of pocket depth (which must be learned throughexperience) can cause severe problems. For example, if the pocket depth istoo shallow, the flash will be squeezed with too much pressure, puttingundue strain on the mold, mold pinchoff areas, and machine-clamp presssection. The molds will be held open, leaving a relatively thick pin-choff, which is difficult to trim properly. If the pocket is too deep, the flashwill not contact the mold surface for proper cooling. In fact, betweenmolding and automatic trimming, heat from the uncooled flash willmigrate into the cool pinchoff and cause it to heat up, creating problemslike sticking to the trimmer. During trimming it can stretch instead ofbreaking free.
The knife-edge cutter width of the pinchoff depends on the resin used,the wall thickness of the blown part, the size of the relief angle, the closingspeed, and the time when blowing starts. As a general guide for smallparts up to 10 mil (250 jam), the width is 4-12 mil (100-300 MJU). Whenprocessing LDPE, one uses the narrowest edge. Edge tapering can help,starting from the center. Its internal edge should be machined smooth andpossibly broken slightly to prevent surface damage of the parison or themolded part during closing and opening. Such surface damage couldinclude dull patches next to the weld line or scratches and scoring duringejection.
Deflashing is not as easy with engineering resin products as with PEs.Even if the processor maximizes the clamping force and the design ofpinchoff edges, conventional methods such as knockingoff, punching, orcutting can be a problem for most production operations. For these plas-tics, other cutting methods are generally used, such as mechanical separa-tion, water-jet cutting, or laser-beam cutting. Robots are used to handlethese types of cutters.
Figure 4.17 Typical pinchoff double-angle design.
Blowing the parison
The air used for blowing serves to expand the parison tube against thewalls of the mold cavity, forcing the melt to assume the shape of the moldand forcing it into the surface details, such as raised letters and surfacedesigns (Table 4.5). The air performs three functions: it expands theparison against the mold, exerts pressure on the expanded parison toproduce surface details, and aids in cooling the blown parison. During theexpansion phase of the blowing process, it is desirable to use the largestavailable volume of air, so the parison is expanded against the mold wallsin the shortest possible time. A maximum volumetric flow rate into thecavity at a low linear velocity can be achieved by making the air-inletorifice as large as possible.
A blow pin is usually located opposite the pinched end of the parison.However, the pins can be located in any position and usually around themold parting line. Various techniques are used. Air can enter through theextrusion die mandrel (as with most pipe lines, Chapter 3), through ablow pin over which the end of a parison has dropped (Fig. 4.8), orthrough blowing needles that pierce the parison. It is possible to avoid theblow-pin mark when using EBM by employing hypodermic needles andpulling them out before the material solidifies.
Blowing inside the neck is sometimes difficult. Small orifices may createa venturi effect, producing a partial vacuum in the tube and causing it tocollapse. If the linear velocity of the incoming blow air is too high, its forcecan actually draw the parison away from the extrusion head end of themold, producing an unblown parison. The air velocity must be carefullyregulated by control valves placed as close as possible to the outlet of theblow tube. The gauge pressure of the air used to inflate commodity andengineering resin parisons is normally about 90psi (0.62MPa) with range30-300psi (0.21-2.1 MPa). Too high a blow pressure will often 'blow out'
Table 4.5 Guide for air blowing pressure
Plastic Pressure (psi)
Acetal 100-150PMMA 50-80PC 70-150LDPE 20-60HDPE 60-100PP 75-100PS 40-100PVC (rigid) 75-100ABS 50-150
the parison. Too little pressure will yield end products lacking adequatesurface details. As high a blowing pressure as possible is desirable to giveboth minimum blow time (therefore higher production rates) and finishedparts that reproduce the mold surface. The optimum blowing pressure isgenerally found by experimentation on the machine that will be used inproduction. The blow pin should not be so long that air is blown againstthe hot plastic opposite the air outlet. That action can create freeze-off andstresses in the container at that point.
Air is a fluid, just like the parison, and as such it has a limited ability toblow through an orifice. If the air-entrance channel is too small, the re-quired blow time will be excessive, or the pressure exerted on the parisonwill not be adequate to reproduce the surface details in the mold. Generalguidelines for determining the optimum diameter of the air-entranceorifice during blowing are (1) up to 1 quart (0.95dm"3) use V16 in. (1.6mm);(2) for 1 quart to 1 gallon (0.95-3.8 dm"3), use 0.25 in. (6.4mm); and (3) for1-54 gallons (3.8-205 dm"3) use 0.5 in. (12.7mm).
The pressure of the blowing air will cause variations in the surfacedetail of the molded items. Some PEs with heavy walls can be blownwith air pressure as low as 30-40 psi (210-28OkPa). Low pressure canbe used because items with heavy walls cool slowly, giving the resinmore time, at a lowered viscosity, to flow into the indentations of themold surface. Thin walls cool rapidly; so the plastic reaching the moldsurface will have a high melt viscosity, and higher pressures will berequired, 50-100psi (0.3-0.7MPa). Larger items such as !gallon contain-ers require a higher air pressure, 100-150psi (0.7-1 .OMPa). The plastic hasto expand farther and takes longer to get to the mold surface in largeritems. During this time the melt heat will drop slightly, producing a moreviscous mass, which requires more air pressure to reproduce the details ofthe mold.
A high volumeteric airflow at a low linear velocity is desired. A highvolumetric flow gives the parison a minimum time to cool before comingin contact with the mold, and provides a more uniform rate of expansion.A low linear velocity is desirable to prevent a venturi effect (seeabove). Volumetric flow is controlled by the line pressure and the orificediameter. Linear velocity is controlled by flow-control valves close to theorifice.
The blowing time differs from the cooling time, being much shorterthan the time required to cool the thickest section to prevent distortion onejection. The blow time for an item may be computed from Table 4.6 andthe following formula:
Mold volume (m3) Final mold pressure (kPa) - 101 kPaBlow time (s) = ^ '- x *- ^ J-
v ; mV1 101 kPa
Table 4.6 Discharge of air at 14.7psi (101 kPa) and 7O0F (210C)
Discharge of air (ft3s~2) for specified orifice diameterGauge 1I16In. 1I8In, 1IJn. 1J2In.pressure (psi) (1.6mm) (3.2mm) (6.4mm) (12.7mm)
5 0.993 3.97 15.9 73.515 1.68 6.72 26.9 10730 2.53 10.1 40.4 16240 3.10 12.4 49.6 19850 3.66 14.7 58.8 23580 5.36 21.4 85.6 342
100 6.49 26.8 107.4 429
This is for free air; but there will be a pressure buildup as the parison isinflated, so the blow rate has to be adjusted. The value of Ui3S'1 is obtainedfrom Table 4.5, according to the line pressure and the orifice diameter. Thefinal mold pressure is assumed to be the line pressure for purposes ofcalculation. Actually, the blow air is heated by the mold, raising its pres-sure. Calculations ignoring this heat effect will be satisfactory when blowtimes are under one second (for small to medium-size parts); but if blowtimes are longer, the air will have time to pick up heat, causing a morerapid pressure buildup and blow times shorter than calculated.
Processors often employ methods to speed up cooling. For example,postcooling of blow-molded parts can shorten the blow cycle. Shuttlemachines, which maximize production in continuous EBM, are preferredby many molders because they can produce finished containers in themachine; but trimming cannot proceed until the scrap areas, the thickestareas of the part, have been cooled sufficiently, so the cycle depends ongetting parts cool enough to trim. If trimming is not done in the machine,the parts can be demolded when they are cool enough to maintain theirshape. Wheel machines are sized to do the job by mounting a sufficientnumber of mold stations to provide adequate cooling for each blowncontainer as it takes its turn around the wheel.
Resins vary in cooling requirements. It is not usually necessaryto postcool PVC; it gives up its heat much more readily than the poly-olefins (making it more appropriate for a dedicated operation than forcustom blow molding). Also the bigger the part, the more cost-effective itscooling.
Postcooling can be extremely beneficial when directed at the thickestareas, especially at pinchoff, neck finish, and thick handle areas.
Prepostcooling is very important in developing any 'fast' cooling con-
trol. It originates with the proper placement of cooling lines in the molds.Unfortunately most blow molds are inefficiently designed for maximizingcooling rates. Improvements are gradually developing, similar to thoseavailable for injection molds [I]. In fact, a few computer-aided designprograms have been produced just for blow-mold cooling analysis.
Efficient mold cooling also depends on accurate venting. Air trappedbetween the mold cavity and the plastic will significantly slow downcooling and also could cause problems with the part. Certain molds incor-porate vacuum lines to ensure proper contact.
Unfortunately, it is not always possible to run the mold as cold aspossible because of a high ambient dew point. With high humidity, themold sweats, causing the surface of a blown part to be damaged. Moldsweating is easily solved by increasing the mold heat, which in turnincreases the cycle time. To eliminate the problem and keep the cycle timeshort, as in other processes, the mold is enclosed in a dry air curtain. Oneshould also consider dehumidifying the room, or just the molding ma-chine in an enclosure or tent, if practical.
As much as 80% of the blow molding cycle is cooling time. Severalmethods are used to reduce cycle time. A part is normally cooled exter-nally by the mold cavity, forcing heat to travel through the entire wallthickness. With the relatively poor thermal conductiv